Ciriottiite , Cu ( Cu , Ag ) 3 Pb 19 ( Sb , As ) 22 ( As 2 ) S 56 , the Cu-Analogue of Sterryite from the Tavagnasco Mining District , Piedmont , Italy

The new mineral species ciriottiite, ideally Cu(Cu,Ag)3Pb19(Sb,As)22(As2)S56 has been discovered in the Tavagnasco mining district, Piedmont, Italy, as very rare black metallic tubular crystals, up to 150 μm in length, associated with Bi sulfosalts and arsenopyrite. Its Vickers hardness (VHN10) is 203 kg/mm2 (range 190–219). In reflected light, ciriottiite is light grey in color, distinctly anisotropic with brownish to greenish rotation tints. Internal reflections are absent. Reflectance values for the four COM wavelengths (Rmin, Rmax (%) (λ in nm)) are: 33.2, 37.8 (471.1); 31.8, 35.3 (548.3), 31.0, 34.7 (586.6); and 27.9, 32.5 (652.3). Electron microprobe analysis gave (in wt %, average of 5 spot analyses): Cu 2.33 (8), Ag 0.53 (5), Hg 0.98 (6), Tl 0.78 (3), Pb 44.06 (14), As 4.66 (7), Sb 23.90 (10), Bi 1.75 (7), total 99.38 (26). On the basis of 56 S atoms per formula unit, the chemical formula of ciriottiite is Cu3.23(11)Ag0.43(4)Hg0.43(2)Pb18.74(9)Tl0.34(1)Sb17.30(5)As5.48(10)Bi0.74(3)S56. The main diffraction lines, corresponding to multiple hkl indices, are (d in Å (relative visual intensity)): 4.09 (m), 3.91 (m), 3.63 (vs), 3.57 (m), 3.22 (m), 2.80 (mw), 2.07 (s). The crystal structure study revealed ciriottiite to be monoclinic, space group P21/n, with unit-cell parameters a = 8.178 (2), b = 28.223 (6), c = 42.452 (5) Å, β = 93.55 (2) ̋, V = 9779.5 (5) Å3, Z = 4. The crystal structure was refined to a final R1 = 0.118 for 21304 observed reflections. Ciriottiite is the Cu analogue of sterryite and can be described as an expanded derivative of owyheeite. The name ciriottiite honors Marco Ernesto Ciriotti (b. 1945) for his longstanding contribution to mineral systematics.


Introduction
During the study of the mineral assemblage of the Pb-Bi-Zn-As-Fe-Cu ore district from Tavagnasco, Turin, Piedmont, Italy, several lead sulfosalts have been identified as accessory minerals.One specimen collected at the Espérance superiore tunnel (latitude 45.5416 N; longitude 7.8134 E) showed tubular crystals, up to 150 µm in length, in the vugs of quartz-carbonate veins.X-ray single-crystal diffraction study indicated a sterryite-like unit-cell, with a smaller unit-cell volume.Chemical analysis and the crystal structure refinement allowed the identification of this phase as the Cu-analogue of sterryite, ideally Cu(Cu,Ag) 3 Pb 19 (Sb,As,Bi) 2 (As 2 )S 56 .This new mineral was named ciriottiite, in honor of Marco Ernesto Ciriotti (b. 1945), Italian member of the IMA CNMNC since 2013, president of the AMI (Associazione Micromineralogica Italiana, Italian Micromineralogical Association) since 2003, for his since 2003, for his contribution to mineral systematics.In addition, he is Associate Editor of MICRO (the AMI magazine) and coauthors of several papers on systematic and topographic mineralogy, and the book "Italian Type Minerals" [1].The mineral and its name have been approved by the IMA CNMNC, under the number 2015-027 [2].The holotype specimen of ciriottiite is deposited in the mineralogical collections of the Museo di Storia Naturale, Università degli Studi di Firenze, Via G. La Pira 4, Florence, Italy, under catalogue number 3161/I.
The mineralogical description of ciriottiite, as well as its crystal structure, are described in this paper.

Geological Setting and Occurrence of Ciriottiite
The geological setting of the Tavagnasco Pb-Bi-Zn-As-Fe-Cu hydrothermal ore district, located about 50 km N of Turin, has been discussed in [3].Ciriottiite occurs in a complex sulfide assemblage.The ore minerals are represented by chalcopyrite, arsenopyrite, galena, with minor amounts of bismuthinite, sulfosalts (cosalite, izoklakeite-giessenite, and a kobellite-like mineral), bismuth, and gold.A series of alteration minerals (anglesite, azurite, langite, and tavagnascoite) have been identified.Ciriottiite is exceptionally rare.Up to now, only one specimen has been identified.In the holotype specimen, ciriottiite is associated with arsenopyrite and a kobellite-like mineral, within a vug of a quartz vein.

Mineral Description and Physical Properties
Ciriottiite (Figure 1) occurs as black tubular crystals, up to 150 μm in length and few μm thick.Streak is black and the luster is metallic.In plane-polarized incident light, ciriottiite is light grey in color.Under crossed polars, it is distinctly anisotropic, with brownish to greenish rotation tints.Internal reflections are absent and there is no optical evidence of growth zonation.Reflectance was measured in air using a Zeiss MPM-200 microphotometer (CRAIC Technologies, San Dimas, CA, USA) equipped with a MSP-20 system processor on a Zeiss Axioplan ore microscope.The filament temperature was approximately 3350 K. Readings were taken for specimen and standard (SiC) maintained under the same focus conditions.The diameter of the circular measuring area was 0.1 mm.Reflectance percentages in the form (Rmin, Rmax (%) (λ in nm)) are: 33.2, 37.8 (471.1);31.8,35.3 (548.3),31.0,34.7 (586.6); and 27.9, 32.5 (652.3).Such values are compared in Figure 2 to those measured on sterryite [4] and parasterryite [5].In plane-polarized incident light, ciriottiite is light grey in color.Under crossed polars, it is distinctly anisotropic, with brownish to greenish rotation tints.Internal reflections are absent and there is no optical evidence of growth zonation.Reflectance was measured in air using a Zeiss MPM-200 microphotometer (CRAIC Technologies, San Dimas, CA, USA) equipped with a MSP-20 system processor on a Zeiss Axioplan ore microscope.The filament temperature was approximately 3350 K. Readings were taken for specimen and standard (SiC) maintained under the same focus conditions.The diameter of the circular measuring area was 0.1 mm.Reflectance percentages in the form (R min , Figure 2. Reflectance values for ciriottiite (this study), sterryite [4] and parasterryite [5].
Ciriottiite is brittle.Its Vickers hardness (VHN10) is 203 kg/mm 2 (range 190-219), corresponding to a Mohs hardness of ~3-3.5.On the basis of the empirical formula, the calculated density is 5.948 g/cm 3 .The density on the basis of the ideal chemical formula is 5.918 g/cm 3 .

Chemical Data
A preliminary EDS (Energy Dispersive Spectrometry) analysis performed on the crystal grain used for the structural study did not indicate the presence of elements (Z > 9) other than Cu, Pb, Bi, Sb, As, and S.

Chemical Data
A preliminary EDS (Energy Dispersive Spectrometry) analysis performed on the crystal grain used for the structural study did not indicate the presence of elements (Z > 9) other than Cu, Pb, Bi, Sb, As, and S.

Crystallography
For the X-ray single-crystal diffraction study, the intensity data were collected using an Oxford Diffraction Xcalibur 3 diffractometer, equipped with a Sapphire 2 CCD area detector, with Mo Kα radiation.The detector to crystal working distance was 6 cm.Intensity integration and standard Lorentz-polarization corrections were performed with the CrysAlis RED [6] software package.The program ABSPACK in CrysAlis RED [6] was used for the absorption correction.Tests on the distribution of |E| values agree with the occurrence of an inversion centre (|E 2 ´1| = 0.927).This information, together with the systematic absences, suggested the space group P2 1 /n.We decided to keep this non-standard setting of the space group to make easier the comparison with sterryite (see below).The refined unit-cell parameters are a = 8.178 ( 2), b = 28.223( 6), c = 42.452(5) Å, β = 93.55(2) ˝, V = 9779.5(5) Å 3 .
The crystal structure was refined with Shelxl-97 [7] starting from the atomic coordinates of sterryite [8], which represents the Ag-analogue of ciriottiite.The site occupancy factors (s.o.f.) were refined using the scattering curves for neutral atoms given in the International Tables for Crystallography [9].Crystal data and details of the intensity data collection and refinement are reported in Table 2.After several cycles of isotropic refinement, the R 1 converged to 0.19, thus confirming the correctness of the structural model.Forty-seven cation and fifty-six anion sites occur in the crystal structure of ciriottiite.Mixed (Pb/Sb) and (Sb/As) sites have been detected, as well as mixed (Cu,Ag,Hg), (Cu,Hg), and (Cu/Bi) sites.The s.o.f. of the Ag34 site was identical to that observed in sterryite, being a mixed (Cu,Ag,Hg) site.Cu is the dominant cation at the former Ag25 of sterryite (now the site is labelled Cu25), probably partially substituted by Hg; Cu is also present at the former Minerals 2016, 6, 8 5 of 12 split Ag33 site of sterryite (now the site is labelled Cu33), partially replaced by Bi.Bismuth was, moreover, attributed to the Pb7 site, the smallest Pb site in the ciriottiite structure.Thallium was not located, but it is likely hosted at one of the largest Pb sites (i.e., Pb1-Pb6 sites).Refining the crystal structure assuming an anisotropic model for cations (but for the Cu33a/Bi33b split pair that resulted negatively defined), the R 1 dropped to 0.12.Finally, the refinement converged to 0.118 for 21304 observed reflections with (F o > 4σ (F o )) assuming the anisotropic displacement parameters for all the atom positions (with the exception of the split pair Cu33a/Bi33b).Notwithstanding a good refinement of all the atom positions, including the lighter ones (S atoms), and reasonable bond distances, the residual factor R remained rather high, with relatively high residuals in the difference-Fourier map.A similar situation was observed in sterryite [8], as well as in other complex lead sulfosalts (see Table 2 in [8]), and probably reflects substitution issues.
The crystal structure refinement pointed to the crystal chemical formula Cu 0.80 (Cu This formula is not perfectly charge-balanced, showing an excess of charges (Ev (%) = +0.70),probably related to the non-localization of minor Tl + , assumed as Pb 2+ owing to the very similar scattering factor.With respect to the chemical data, the formula derived through the crystal structure refinement shows a lower Cu content (2.73 apfu, to be compared with 3.23 apfu from electron-microprobe analysis) and a lower Sb/As atomic ratio (2.72 to be compared with 3.15).Finally, a lower amount of Bi has been localized, even if some additional Bi could be hosted at Pb8 (~0.2 Bi apfu).
In order to propose an ideal chemical formula for ciriottiite, the occurrence of 0.34 apfu Tl replacing Pb cannot be neglected.
Consequently, the chemical formula derived from the crystal structure refinement could be conveniently written as Cu 0.80 (Cu The X-ray powder diffraction pattern, based on this structural model and calculated using the software PowderCell 2.3 [10], is given in Table 3. Owing to the uniqueness of the available crystal used for the single-crystal X-ray diffraction study and to the fact it was subsequently embedded in epoxy and polished for electron-microprobe analysis, X-ray powder pattern was not collected.

General Features
Owing to the large number of independent atom positions in the unit-cell, atom coordinates and displacement parameters for ciriottiite are given in the CIF, available as Supplementary material.
The crystal structure of ciriottiite is topologically identical with that of sterryite [8].It is composed by the fishbone arrangement of complex columns along b.These complex columns have been delimited by dotted lines in Figure 3 and they have been defined taking into account the surfaces of weakest bonding, cutting the longest (Sb/As)-S bonds along distinct lone-electron-pair micelles.A single kind of complex column, corresponding to one unit formula, occurs in ciriottiite.It has a pseudotrigonal prismatic core and two "arms" (=ribbon projections) of unequal length (Figure 4), i.e., short and long arms.Each complex column contains 16 Pb sites (with minor Bi and Tl), 10 pure Sb sites, 10 mixed (Sb/As) sites (five having As > Sb), and five mixed (Pb/Sb) positions (one having Sb > Pb).
As in sterryite, one of the mixed (Pb,Sb) position (i.e., Pb44) located on the short arm is connected to a partially occupied Cu site (i.e., Cu43) in such a way that the Cu s.o.f.(0.80) is very close to the Pb s.o.f.(0.81), corresponding to the substitution rule Pb44 Pb 2+ + Cu43 Cu + = Pb44 Sb 3+ + Cu43 γ.In the short arm there are two pure As sites, forming localized As-As bonds characterizing both ciriottiite and sterryite (Figure 4a).A single kind of complex column, corresponding to one unit formula, occurs in ciriottiite.It has a pseudotrigonal prismatic core and two "arms" (=ribbon projections) of unequal length (Figure 4), i.e., short and long arms.Each complex column contains 16 Pb sites (with minor Bi and Tl), 10 pure Sb sites, 10 mixed (Sb/As) sites (five having As > Sb), and five mixed (Pb/Sb) positions (one having Sb > Pb).
As in sterryite, one of the mixed (Pb,Sb) position (i.e., Pb44) located on the short arm is connected to a partially occupied Cu site (i.e., Cu43) in such a way that the Cu s.o.f.(0.80) is very close to the Pb s.o.f.(0.81), corresponding to the substitution rule Pb44 Pb 2+ + Cu43 Cu + = Pb44 Sb 3+ + Cu43 γ.In the short arm there are two pure As sites, forming localized As-As bonds characterizing both ciriottiite and sterryite (Figure 4a).
The other Cu-hosting sites are located in the long arm.At its base, a mixed and split (Cu/Bi) site, namely Cu33, alternates with a mixed (Cu,Ag,Hg) site (Cu34); the former corresponds to a split (Cu/Ag) site in sterryite [8] (Figure 4b).At the end of the long arm, a (Cu,Hg) site (Cu25) alternates with a mixed (Sb,As) site (Sb26) (Figure 4c); in sterryite, as well as in parasterryite and meerschautite [8,11], a similar configuration with an (Ag,Cu) site alternating with an Sb one was reported [8].
As in the crystal structure descriptions of sterryite and parasterryite [8], each column has been delimited by three faces denoted A, B, and C (more details in [8]); these different faces control the polymerization of (Sb/As) sites with S. The other Cu-hosting sites are located in the long arm.At its base, a mixed and split (Cu/Bi) site, namely Cu33, alternates with a mixed (Cu,Ag,Hg) site (Cu34); the former corresponds to a split (Cu/Ag) site in sterryite [8] (Figure 4b).At the end of the long arm, a (Cu,Hg) site (Cu25) alternates with a mixed (Sb,As) site (Sb26) (Figure 4c); in sterryite, as well as in parasterryite and meerschautite [8,11], a similar configuration with an (Ag,Cu) site alternating with an Sb one was reported [8].
As in the crystal structure descriptions of sterryite and parasterryite [8], each column has been delimited by three faces denoted A, B, and C (more details in [8]); these different faces control the polymerization of (Sb/As) sites with S.

Cation Coordination and Site Occupancies
Owing to the large number of Pb, Sb, and As sites occurring in the crystal structure of ciriottiite, their coordination will be not detailed here.Pb sites display a coordination number ranging from 6 to 9, as in sterryite [8].The bond-valence sums (BVS) for pure Pb sites, calculated using the bond parameters given in [12] and expressed in valence unit (v.u.), range between 1.89 (Pb30) and 2.43 v.u.(Pb7).The oversaturation of the latter was interpreted as due to minor Bi replacing Pb and the s.o.f.(Pb0.60Bi0.40)was assumed; minor amounts of Bi could additionally be hosted at the Pb8 site, having a BVS of 2.25 v.u.Sb and As sites usually show a triangular pyramidal coordination (taking into account only the shortest Me-S distances); their BVSs range between 2.75 (Sb29) and 3.60 v.u.(Sb42).In ciriottiite, these sites usually result overbonded; following the bond-valence method used during the crystal structure study of sterryite and parasterryite [8], this oversaturation could indicate the occurrence of an As content larger than those found both during electron-microprobe analysis and crystal structure refinement, i.e., ca.6.9As apfu.Mixed (Pb/Sb) sites display usually a six-fold coordination; if split, the Sb position usually has only two distances shorter than 2.70 Å, as a result of its average position.
In the short arm, the Cu43 site has a distorted tetrahedral coordination, with three short distances ranging between 2.25 and 2.30 Å, and a longer one at 2.57 Å.Its BVS, calculated assuming the refined s.o.f., is 0.89 v.u.In the same arm, the As46 and As47 sites are at short distance along a, i.e., 2.63 Å, forming an As-As pair.Each As atom of this pair is bonded to two S atoms, thus forming an (As2)S4 group, analogous to that occurring in sterryite [8] and similar to those reported in several As sulfides (e.g., alacranite [13], bonazziite [14], realgar [15], uzonite [16], wakabayashilite [17]) and in dervillite [18].

Cation Coordination and Site Occupancies
Owing to the large number of Pb, Sb, and As sites occurring in the crystal structure of ciriottiite, their coordination will be not detailed here.Pb sites display a coordination number ranging from 6 to 9, as in sterryite [8].The bond-valence sums (BVS) for pure Pb sites, calculated using the bond parameters given in [12] and expressed in valence unit (v.u.), range between 1.89 (Pb30) and 2.43 v.u.(Pb7).The oversaturation of the latter was interpreted as due to minor Bi replacing Pb and the s.o.f.(Pb 0.60 Bi 0.40 ) was assumed; minor amounts of Bi could additionally be hosted at the Pb8 site, having a BVS of 2.25 v.u.Sb and As sites usually show a triangular pyramidal coordination (taking into account only the shortest Me-S distances); their BVSs range between 2.75 (Sb29) and 3.60 v.u.(Sb42).In ciriottiite, these sites usually result overbonded; following the bond-valence method used during the crystal structure study of sterryite and parasterryite [8], this oversaturation could indicate the occurrence of an As content larger than those found both during electron-microprobe analysis and crystal structure refinement, i.e., ca.6.9As apfu.Mixed (Pb/Sb) sites display usually a six-fold coordination; if split, the Sb position usually has only two distances shorter than 2.70 Å, as a result of its average position.
In the short arm, the Cu43 site has a distorted tetrahedral coordination, with three short distances ranging between 2.25 and 2.30 Å, and a longer one at 2.57 Å.Its BVS, calculated assuming the refined s.o.f., is 0.89 v.u.In the same arm, the As46 and As47 sites are at short distance along a, i.e., 2.63 Å, forming an As-As pair.Each As atom of this pair is bonded to two S atoms, thus forming an (As 2 )S 4 group, analogous to that occurring in sterryite [8] and similar to those reported in several As sulfides (e.g., alacranite [13], bonazziite [14], realgar [15], uzonite [16], wakabayashilite [17]) and in dervillite [18].
The two Cu sites located at the base of the long arm, i.e., Cu33 and Cu34, have mixed occupancies.Cu33 is actually split into two sub-positions, Cu33a and Bi33b.Cu33a has a coordination close to a linear one, with two S atoms at 2.43 and 2.44 Å.Other two S atoms are located at 2.77 and 2.89 Å; the Cu33a coordination is completed by two additional S at 3.08 and 3.10 Å.The Bi33b position has been tentatively assigned to Bi.The coordination environment can be described as a distorted octahedron, with distances ranging from 2.47 to 3.46 Å.Actually, a Bi-S distance of 2.47 Å is too short and results in an oversaturation of the Bi atom at the Bi33b position (4.22 v.u.instead of the theoretical 3.00 v.u.).In our opinion, the positions of the S atoms bonded to the split pair Cu33a/Bi33b are only average positions.Indeed, assuming a full-occupancy of Cu at the Cu33a site, a BVS of 0.64 v.u. is obtained, thus indicating a too large site for a pure Cu site.Assuming mixed (Cu,Bi) population, the weighted BVS is 1.35 v.u., to be compared with a theoretical value of 1.40 v.u.calculated on the basis of the refined s.o.f.(Cu 0.80 Bi 0.20 ).Cu34 corresponds to a mixed (Cu,Ag,Hg) site, as in sterryite [8].It displays two short distances (Me-S distances of 2.48 and 2.58 Å), arranged in a linear coordination, and four additional longer ones (three ranging between 2.81 and 2.96 Å, and a fourth one at 3.22 Å).This polyhedron is similar to that reported in sterryite [8]; the average <Cu34-S> distance is 2.81 Å.The BVS at the Cu34 site is 1.10 v.u.; the theoretical value, calculated on the basis of the assumed s.o.f.(Cu 0.40 Ag 0.40 Hg 0.20 ) should be 1.20 v.u.
At the end of the long arm, Cu25 site displays a strongly distorted octahedral coordination, close to a linear one.Indeed, two S atoms are at 2.39 and 2.43 Å from the metal position; other two are located at 2.64 and 2.74.The remaining S atoms are at very long distances, i.e., 3.53 and 3.58 Å.The site occupancy at Cu25 has been interpreted as a mixed (Cu,Hg).The BVS is 1.15 v.u., to be compared with the theoretical value 1.27 v.u.calculated on the basis of the refined s.o.f.(Cu 0.73 Hg 0.27 ).

Polymerization of (Sb/As) Sites
The examination of the organization of the (Sb/As) sites into finite Me 3+ m S n chain fragments (hereafter "polymers") is possible by taking into account only the shortest Me 3+ -S bond distances (Me-S distances shorter than 2.70 Å [8]).
On the face A (Figure 5a), a central squared Me 2 S 4 group (where Me = Sb 1.92 As 0.08 ), is edged by two MeS 3 groups, with Me = (Sb 0.66 As 0.34 ) and (As 0.58 Sb 0.42 ), respectively.
On sub-surface B1 (Figure 5b), there are two peripheral MeS 3 groups, with Me having composition (As 0.72 Sb 0.28 ) and Sb, respectively.The central portions are formed by two distinct polymers.One of the sites involved in these polymers is actually a mixed (Sb,Pb) site.If Pb is absent, there are two open Me 2 S 4 groups, with Me = (Sb 1.36 As 0.64 ) and Sb 2.00 , respectively.On the contrary, if Pb occurs, the central portion of the B1 sub-surface shows an Me 2 S 4 polymer and an isolated SbS 3 group.
On sub-surface B1 (Figure 5b), there are two peripheral MeS3 groups, with Me having composition (As0.72Sb0.28)and Sb, respectively.The central portions are formed by two distinct polymers.One of the sites involved in these polymers is actually a mixed (Sb,Pb) site.If Pb is absent, there are two open Me2S4 groups, with Me = (Sb1.36As0.64)and Sb2.00, respectively.On the contrary, if Pb occurs, the central portion of the B1 sub-surface shows an Me2S4 polymer and an isolated SbS3 group.3 and 4.
Along the C1 sub-surface (Figure 6a), an asymmetric sequence of MeS 3 , open Me 2 S 4 , and a crankshaft chain Me 3 S 7 .
The (Sb/As) m S n polymers in the outer part of the long arm concerns the two atom sub-surfaces B2 and C2 (Figure 6b).In ciriottiite, there are three mixed (Pb,Sb) positions (Pb22, Pb23, and Pb27).Neglecting the minor Sb content of these sites, three Me m S n groups can be highlighted, i.e., MeS Along the C1 sub-surface (Figure 6a), an asymmetric sequence of MeS3, open Me2S4, and a crankshaft chain Me3S7.Me occupancies correspond to Sb, (Sb1.93As0.07),and (Sb1.66As1.34),respectively.
The (Sb/As)mSn polymers in the outer part of the long arm concerns the two atom sub-surfaces B2 and C2 (Figure 6b).In ciriottiite, there are three mixed (Pb,Sb) positions (Pb22, Pb23, and Pb27).Neglecting the minor Sb content of these sites, three MemSn groups can be highlighted, i.e., MeS3, a stretched Me2S4, and a Me2S5 group, with Me corresponding to Sb, Sb2.00, and (Sb1.40As0.60),respectively.Such a polymeric organization closely corresponds to that reported for sterryite [8].

Ciriottiite in the Framework of the Owyheeite Group and Its Comparison with Sterryite
Ciriottiite is the Cu-analogue of sterryite, Cu(Ag,Cu)3Pb19(Sb,As)22(As2)S56.It is an expanded derivative of owyheeite, belonging to the owyheeite group (Table 4).Such a polymeric organization closely corresponds to that reported for sterryite [8].All these sulfosalts are characterized by crystal structures built around a pseudotrigonal core, relating them to the zinkenite plesiotypic series (sulfosalts of the cyclic rod-type and derivatives [22,23]).
The substitution of Cu for Ag was reported in sterryite from the Pollone mine.Indeed, two chemical varieties were described, i.e., Sb-rich and Sb-poor sterryite.Actually, the Sb-rich sterryite is also Cu-rich, with a Cu/(Cu + Ag + Hg) atomic ratio of 0.464.to be compared with 0.230 in Sb-poor sterryite.Ciriottiite is definitely enriched in Cu, with a Cu/(Cu + Ag + Hg) atomic ratio of 0.788.The As/(As + Sb + Bi) atomic ratio is 0.240, close to the value reported for Sb-rich sterryite, i.e., 0.259; Sb-poor sterryite is As-enriched, with an As/(As + Sb + Bi) atomic ratio of 0.392.Consequently, ciriottiite appears as being a Cu-dominant Sb-rich sterryite.This chemical difference is reflected in the smaller unit-cell volume of the former, showing a volume contraction of ca.´2.25%, probably as result of the substitution of Ag with Cu, having a smaller atomic radius (1.00 vs. 0.60 Å, respectively).

The Study of Sulfosalts as a Proxy for Unraveiling Ore Geochemistry
Sulfosalts are a heterogeneous group of compounds relatively common as accessory minerals in hydrothermal veins.Many species have very complex chemistry and in some cases minor chemical components appear fundamental for their stabilization.Only an accurate knowledge of their crystal structures allows the understanding of the role of such minor components in these compounds, giving interesting insights into the ore geochemistry.Indeed, the crystal chemistry of the sulfosalts occurring in a hydrothermal vein is mainly controlled by the chemistry of the hydrothermal fluids.Therefore, the characterization of sulfosalt assemblage could give interesting information about the ore geochemistry.In other cases, some structural features could indicate particular crystallization conditions, like the presence of chlorine site (e.g., dadsonite [24]), indicating the high chlorinity of the hydrothermal solutions, or localized S-S bonds, indicating high f (S 2 ) conditions (e.g., moëloite [25]).
The occurrence of the As-As pair in ciriottiite, revealed through the crystal structure solution, indicates a S deficit, i.e., a low f (S 2 ) in the crystallization medium; probably, such a relatively low f (S 2 ) allows the stabilization of ciriottiite, explaining its extreme rarity in nature, as hypothesized for sterryite [4].In addition, the Cu-rich nature of this new mineral with respect to sterryite is related to the Cu-rich nature of the Tavagnasco ore district, with the occurrence of chalcopyrite as one of most important sulfides forming the ore deposits.Ciriottiite is thus a multicomponent compound belonging ideally to the pseudo-quinary system PbS-Sb 2 S 3 -As 2 S 3 -Cu 2 S-AsS.

Figure 1 .
Figure 1.Backscattered electron image of ciriottiite obtained with a Scanning Electron Microscopy.

Figure 1 .
Figure 1.Backscattered electron image of ciriottiite obtained with a Scanning Electron Microscopy.

Figure 3 .
Figure 3. Projection of the crystal structure of ciriottiite, as seen down a.The fishbone layer along b, formed by the connection of complex columns, is shaded in light blue.Red ellipses (dotted lines) symbolize the lone-electron-pair micelles of (Sb/As) atoms.Red triangles show the pseudotrigonal organization of the prismatic core of the complex columns.Circles: grey = Pb sites; orange = Sb sites; violet = As sites; blue = Cu sites; yellow = S sites.

Figure 3 .
Figure 3. Projection of the crystal structure of ciriottiite, as seen down a.The fishbone layer along b, formed by the connection of complex columns, is shaded in light blue.Red ellipses (dotted lines) symbolize the lone-electron-pair micelles of (Sb/As) atoms.Red triangles show the pseudotrigonal organization of the prismatic core of the complex columns.Circles: grey = Pb sites; orange = Sb sites; violet = As sites; blue = Cu sites; yellow = S sites.

Figure 4 .
Figure 4.The fundamental building block of ciriottiite as seen down a.The pseudo-trigonal rod is highlighted.The A, B1, B2, C1, and C2 faces are shown.Some structural features discussed in the text are shown in (a)-(c).Same symbols as in Figure 3.In addition, light violet circle = Bi site.

Figure 4 .
Figure 4.The fundamental building block of ciriottiite as seen down a.The pseudo-trigonal rod is highlighted.The A, B1, B2, C1, and C2 faces are shown.Some structural features discussed in the text are shown in (a)-(c).Same symbols as in Figure 3.In addition, light violet circle = Bi site.

Figure 5 .
Figure 5. (Sb/As)-S polymerization along the A (a); and B1 (b) surfaces.Shortest (Sb/As)-S bonds are shown as thick red lines; dotted lines represent longer (Sb/As)-S bonds and other Me-S bonds.Circles: same symbols as in Figures 3 and 4.
Figure 5. (Sb/As)-S polymerization along the A (a); and B1 (b) surfaces.Shortest (Sb/As)-S bonds are shown as thick red lines; dotted lines represent longer (Sb/As)-S bonds and other Me-S bonds.Circles: same symbols as in Figures 3 and 4.

Figure 5 .
Figure 5. (Sb/As)-S polymerization along the A (a); and B1 (b) surfaces.Shortest (Sb/As)-S bonds are shown as thick red lines; dotted lines represent longer (Sb/As)-S bonds and other Me-S bonds.Circles: same symbols as in Figures 3 and 4.

Table 2 .
Crystal and experimental details for ciriottiite.

Table 3 .
Calculated X-ray powder diffraction data for ciriottiite.Only reflections with I calc > 10 are listed.The five strongest reflections are given in bold.
3 , a stretched Me 2 S 4 , and a Me 2 S 5 group, with Me corresponding to Sb, Sb 2.00 , and (Sb 1.40 As 0.60 ), respectively.

Table 4 .
Members of the owyheeite group.
Ciriottiite in the Framework of the Owyheeite Group and Its Comparison with SterryiteCiriottiite is the Cu-analogue of sterryite, Cu(Ag,Cu) 3 Pb 19 (Sb,As) 22 (As 2 )S 56 .It is an expanded derivative of owyheeite, belonging to the owyheeite group (Table4).

Table 4 .
Members of the owyheeite group.